#------------------------------------------------------------------------------
#$Date: 2023-11-07 10:11:37 +0200 (Tue, 07 Nov 2023) $
#$Revision: 287467 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/57/02/1570283.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1570283
loop_
_publ_author_name
'Avdontceva, Margarita S.'
'Zolotarev, Andrey A.'
'Shablinskii, Andrey P.'
'Bocharov, Vladimir N.'
'Kasatkin, Anatoly V.'
'Krivovichev, Sergey V.'
_publ_section_title
;
 Galeite, Na15(SO4)5ClF4, and Schairerite, Na21(SO4)7ClF6: Phase
 Transitions, Thermal Expansion and Thermal Stability
;
_journal_issue                   10
_journal_name_full               Symmetry
_journal_page_first              1871
_journal_paper_doi               10.3390/sym15101871
_journal_volume                  15
_journal_year                    2023
_chemical_formula_moiety         'Cl1 F6 Na21 O28 S7'
_chemical_formula_sum            'Cl F6 Na21 O28 S7'
_chemical_formula_weight         1304.66
_space_group_crystal_system      trigonal
_space_group_IT_number           164
_space_group_name_Hall           '-P 3 2"'
_space_group_name_H-M_alt        'P -3 m 1'
_atom_sites_solution_primary     dual
_audit_creation_date             2023-08-26
_audit_creation_method
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6408)
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   7.0714(2)
_cell_length_b                   7.0714(2)
_cell_length_c                   19.5972(7)
_cell_measurement_reflns_used    4435
_cell_measurement_temperature    600.0(4)
_cell_measurement_theta_max      28.7560
_cell_measurement_theta_min      3.3180
_cell_volume                     848.66(5)
_computing_cell_refinement       'CrysAlisPro 1.171.41.104a (Rigaku OD, 2021)'
_computing_data_collection       'CrysAlisPro 1.171.41.104a (Rigaku OD, 2021)'
_computing_data_reduction        'CrysAlisPro 1.171.41.104a (Rigaku OD, 2021)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2014/6 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      600.0(4)
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_detector_type            HyPix
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.932
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
--------------------------------------------------------------------------
  1  ω    -14.00  18.00   0.50    1.50    --   14.80  57.00 -90.00   64
  2  ω    -13.00  42.00   0.50    1.50    --   14.80  19.00   0.00  110
  3  ω    -15.00  34.00   0.50    1.50    --   14.80  57.00  60.00   98
  4  ω    -22.00  42.00   0.50    1.50    --   14.80  38.00-150.00  128
  5  ω    -25.00  43.00   0.50    1.50    --   14.80  19.00 -60.00  136
  6  ω    -14.00  35.00   0.50    1.50    --   14.80  57.00 -30.00   98
  7  ω     -7.00  24.00   0.50    1.50    --   14.80  77.00 120.00   62
  8  ω     -6.00  39.00   0.50    1.50    --   14.80  38.00 120.00   90
  9  ω    -23.00  42.00   0.50    1.50    --   14.80  19.00  60.00  130
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type
'XtaLAB Synergy, Single source at home/near, HyPix'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      0.0546633000
_diffrn_orient_matrix_UB_12      -0.0609985000
_diffrn_orient_matrix_UB_13      0.0014953000
_diffrn_orient_matrix_UB_21      -0.0095839000
_diffrn_orient_matrix_UB_22      -0.0139354000
_diffrn_orient_matrix_UB_23      -0.0359257000
_diffrn_orient_matrix_UB_31      0.1016422000
_diffrn_orient_matrix_UB_32      0.0974682000
_diffrn_orient_matrix_UB_33      -0.0041796000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0231
_diffrn_reflns_av_unetI/netI     0.0125
_diffrn_reflns_Laue_measured_fraction_full 0.994
_diffrn_reflns_Laue_measured_fraction_max 0.932
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            8548
_diffrn_reflns_point_group_measured_fraction_full 0.994
_diffrn_reflns_point_group_measured_fraction_max 0.932
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.449
_diffrn_reflns_theta_min         3.327
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'PhotonJet (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    0.949
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.79201
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.41.104a (Rigaku Oxford Diffraction, 2021)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    2.553
_exptl_crystal_description       plate
_exptl_crystal_F_000             638
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.07
_refine_diff_density_max         1.030
_refine_diff_density_min         -0.732
_refine_diff_density_rms         0.101
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.018
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     96
_refine_ls_number_reflns         910
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.036
_refine_ls_R_factor_all          0.0578
_refine_ls_R_factor_gt           0.0485
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.1102P)²+0.9450P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1602
_refine_ls_wR_factor_ref         0.1697
_reflns_Friedel_coverage         0.000
_reflns_number_gt                741
_reflns_number_total             910
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            schairerite_600K.cif
_cod_data_source_block           sch_600k_auto
_cod_original_cell_volume        848.66(6)
_cod_database_code               1570283
_shelxl_version_number           2014/6
_chemical_oxdiff_formula         'Na21 S7 O28 Cl6 F'
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_reflns_odcompleteness_completeness 99.59
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_olex2_refinement_description
;
1. Restrained distances
 S4-O10 = S4-O12
 1.45 with sigma of 0.02
2. Uiso/Uaniso restraints and constraints
Uanis(O3) = Uanis(O6)
Uanis(O12) = Uanis(O11)
3. Others
 Fixed Sof: O9(0.45) O11(0.2) O4(0.25) O5(0.25) O6(0.083333) O3(0.083333)
 O10(0.083333) O8(0.05) O12(0.05)
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.348
_oxdiff_exptl_absorpt_empirical_full_min 0.775
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
S1 S 0.6667 0.3333 0.35023(7) 0.0228(4) Uani 1 6 d S T P . .
S4 S 0.0000 0.0000 0.5000 0.0296(5) Uani 1 12 d DS T P . .
S3 S 0.6667 0.3333 0.07692(7) 0.0244(4) Uani 1 6 d S T P . .
S2 S 1.0000 1.0000 0.22912(9) 0.0306(4) Uani 1 6 d S T P . .
Cl1 Cl 0.0000 0.0000 0.0000 0.0623(9) Uani 1 12 d S T P A .
Na1 Na 0.5000 0.5000 0.5000 0.0442(7) Uani 1 4 d S T P . .
Na3 Na 0.48618(13) 0.51382(13) 0.22030(8) 0.0404(5) Uani 1 2 d S T P A .
Na2 Na 0.18110(14) 0.3622(3) 0.36492(9) 0.0403(5) Uani 1 2 d S T P . .
Na4 Na 0.18061(16) 0.3612(3) 0.08182(11) 0.0541(6) Uani 1 2 d S T P . .
F2 F 0.3333 0.6667 0.29469(17) 0.0339(8) Uani 1 6 d S T P A .
F1 F 0.3333 0.6667 0.4488(2) 0.0401(9) Uani 1 6 d S T P A .
F3 F 0.3333 0.6667 0.1473(2) 0.0438(10) Uani 1 6 d S T P A .
O1 O 0.5540(2) 0.4460(2) 0.37515(16) 0.0443(7) Uani 1 2 d S T P A .
O2 O 0.6667 0.3333 0.2756(3) 0.0525(14) Uani 1 6 d S T P A .
O7 O 0.6667 0.3333 0.0042(3) 0.074(2) Uani 1 6 d S T P A .
O9 O 0.5547(3) 0.1093(6) 0.1024(2) 0.0654(11) Uani 0.9 2 d S T P A 1
O11 O -0.1137(6) -0.2275(13) 0.5132(6) 0.064(2) Uani 0.4 2 d S T P B 1
O4 O 0.7769(14) 0.8885(7) 0.2076(4) 0.0449(17) Uani 0.5 2 d S T P A 1
O5 O 0.7740(16) 0.8870(8) 0.2439(5) 0.067(3) Uani 0.5 2 d S T P A 2
O6 O 1.0000 1.0000 0.3090(6) 0.074(3) Uani 0.5 6 d S T P A 2
O3 O 1.0000 1.0000 0.1485(6) 0.074(3) Uani 0.5 6 d S T P A 1
O10 O 0.0000 0.0000 0.4203(5) 0.065(3) Uani 0.5 6 d DS T P A .
O8 O 0.464(5) 0.232(2) 0.1177(17) 0.054(8) Uani 0.1 2 d S T P A 2
O12 O -0.1045(18) -0.209(4) 0.4691(19) 0.064(2) Uani 0.1 2 d DS T P A 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Na3 S1 Na3 69.19(5) 3_665 . ?
Na3 S1 Na3 69.19(5) 2_655 . ?
Na3 S1 Na3 69.18(5) 2_655 3_665 ?
O1 S1 Na3 68.53(13) 3_665 3_665 ?
O1 S1 Na3 124.12(10) 3_665 . ?
O1 S1 Na3 124.12(10) 2_655 3_665 ?
O1 S1 Na3 124.12(10) . 3_665 ?
O1 S1 Na3 68.53(13) . . ?
O1 S1 Na3 124.12(10) . 2_655 ?
O1 S1 Na3 124.12(10) 3_665 2_655 ?
O1 S1 Na3 124.12(10) 2_655 . ?
O1 S1 Na3 68.53(13) 2_655 2_655 ?
O1 S1 O1 109.45(13) 3_665 . ?
O1 S1 O1 109.45(13) 3_665 2_655 ?
O1 S1 O1 109.45(13) 2_655 . ?
O2 S1 Na3 40.96(3) . 3_665 ?
O2 S1 Na3 40.96(3) . . ?
O2 S1 Na3 40.96(3) . 2_655 ?
O2 S1 O1 109.49(13) . 3_665 ?
O2 S1 O1 109.49(13) . 2_655 ?
O2 S1 O1 109.49(13) . . ?
O11 S4 O11 116.7(3) 2 . ?
O11 S4 O11 63.3(3) 9_556 . ?
O11 S4 O11 180.0 2 8_556 ?
O11 S4 O11 116.7(3) 3 . ?
O11 S4 O11 180.0(9) 3 9_556 ?
O11 S4 O11 63.3(3) 2 7_556 ?
O11 S4 O11 116.7(3) 8_556 9_556 ?
O11 S4 O11 116.7(3) 8_556 7_556 ?
O11 S4 O11 116.7(3) 2 3 ?
O11 S4 O11 63.3(3) 8_556 3 ?
O11 S4 O11 116.7(3) 7_556 9_556 ?
O11 S4 O11 63.3(3) 7_556 3 ?
O11 S4 O11 180.0 7_556 . ?
O11 S4 O11 63.3(3) 2 9_556 ?
O11 S4 O11 63.3(3) 8_556 . ?
O12 S4 O12 103.1(19) 7_556 9_556 ?
O12 S4 O12 103.1(19) 3 . ?
O12 S4 O12 76.9(19) 8_556 . ?
O12 S4 O12 103.1(19) 2 3 ?
O12 S4 O12 76.9(19) 7_556 3 ?
O12 S4 O12 180.0 7_556 . ?
O12 S4 O12 103.1(19) 2 . ?
O12 S4 O12 76.9(19) 9_556 . ?
O12 S4 O12 180(3) 8_556 2 ?
O12 S4 O12 180(3) 9_556 3 ?
O12 S4 O12 76.9(19) 7_556 2 ?
O12 S4 O12 103.1(19) 7_556 8_556 ?
O12 S4 O12 76.9(19) 8_556 3 ?
O12 S4 O12 103.1(19) 8_556 9_556 ?
O12 S4 O12 76.9(19) 2 9_556 ?
O7 S3 O9 109.96(18) . 2_655 ?
O7 S3 O9 109.97(18) . . ?
O7 S3 O9 109.96(18) . 3_665 ?
O7 S3 O8 122.8(14) . 2_655 ?
O7 S3 O8 122.8(14) . . ?
O7 S3 O8 122.8(14) . 3_665 ?
O9 S3 O9 108.97(18) 2_655 . ?
O9 S3 O9 108.97(18) 2_655 3_665 ?
O9 S3 O9 108.97(18) . 3_665 ?
O8 S3 O8 93(2) 2_655 . ?
O8 S3 O8 93(2) 2_655 3_665 ?
O8 S3 O8 93(2) 3_665 . ?
O4 S2 O4 111.7(3) . 3_675 ?
O4 S2 O4 111.7(3) 3_675 2_765 ?
O4 S2 O4 111.7(3) . 2_765 ?
O4 S2 O3 72.9(3) 2_765 . ?
O4 S2 O3 72.9(3) . . ?
O4 S2 O3 72.9(3) 3_675 . ?
O5 S2 O5 115.9(3) . 3_675 ?
O5 S2 O5 115.9(3) 2_765 . ?
O5 S2 O5 115.9(3) 2_765 3_675 ?
O5 S2 O6 78.2(5) 2_765 . ?
O5 S2 O6 78.2(5) . . ?
O5 S2 O6 78.2(5) 3_675 . ?
Na4 Cl1 Na4 89.04(6) 2 . ?
Na4 Cl1 Na4 90.96(6) 2 9 ?
Na4 Cl1 Na4 180.00(9) 8 2 ?
Na4 Cl1 Na4 89.04(6) 3 . ?
Na4 Cl1 Na4 180.0 7 . ?
Na4 Cl1 Na4 90.96(6) 8 . ?
Na4 Cl1 Na4 90.96(6) 8 3 ?
Na4 Cl1 Na4 180.00(8) 9 3 ?
Na4 Cl1 Na4 90.96(6) 7 3 ?
Na4 Cl1 Na4 89.04(6) 7 8 ?
Na4 Cl1 Na4 90.96(6) 7 2 ?
Na4 Cl1 Na4 89.04(6) 2 3 ?
Na4 Cl1 Na4 90.96(6) 9 . ?
Na4 Cl1 Na4 89.04(6) 8 9 ?
Na4 Cl1 Na4 89.04(6) 7 9 ?
F1 Na1 F1 180.0 . 7_666 ?
F1 Na1 O1 78.95(11) . . ?
F1 Na1 O1 101.05(11) 7_666 . ?
F1 Na1 O1 78.95(11) 7_666 7_666 ?
F1 Na1 O1 101.05(11) . 7_666 ?
F1 Na1 O11 72.40(16) 7_666 2 ?
F1 Na1 O11 72.40(16) . 7_556 ?
F1 Na1 O11 72.40(16) 7_666 1_665 ?
F1 Na1 O11 107.60(16) 7_666 8_666 ?
F1 Na1 O11 107.60(16) 7_666 7_556 ?
F1 Na1 O11 107.60(16) . 2 ?
F1 Na1 O11 72.40(16) . 8_666 ?
F1 Na1 O11 107.60(16) . 1_665 ?
F1 Na1 O12 96.8(6) 7_666 7_556 ?
F1 Na1 O12 83.2(6) 7_666 2 ?
F1 Na1 O12 96.8(6) 7_666 8_666 ?
F1 Na1 O12 83.2(6) 7_666 1_665 ?
F1 Na1 O12 83.2(6) . 8_666 ?
F1 Na1 O12 96.8(6) . 1_665 ?
F1 Na1 O12 96.8(6) . 2 ?
F1 Na1 O12 83.2(6) . 7_556 ?
O1 Na1 O1 180.00(7) 7_666 . ?
O1 Na1 O12 106.9(7) 7_666 2 ?
O1 Na1 O12 106.9(7) . 8_666 ?
O1 Na1 O12 73.1(7) 7_666 8_666 ?
O1 Na1 O12 73.1(7) 7_666 7_556 ?
O1 Na1 O12 73.1(7) . 1_665 ?
O1 Na1 O12 106.9(7) 7_666 1_665 ?
O1 Na1 O12 73.1(7) . 2 ?
O1 Na1 O12 106.9(7) . 7_556 ?
O11 Na1 O1 91.6(3) 1_665 . ?
O11 Na1 O1 88.4(3) 2 7_666 ?
O11 Na1 O1 91.6(3) 2 . ?
O11 Na1 O1 88.4(3) 7_556 . ?
O11 Na1 O1 88.4(3) 1_665 7_666 ?
O11 Na1 O1 91.6(3) 8_666 7_666 ?
O11 Na1 O1 88.4(3) 8_666 . ?
O11 Na1 O1 91.6(3) 7_556 7_666 ?
O11 Na1 O11 144.6(3) 7_556 8_666 ?
O11 Na1 O11 144.6(3) 1_665 2 ?
O11 Na1 O11 180.0 8_666 2 ?
O11 Na1 O11 35.4(3) 7_556 2 ?
O11 Na1 O11 35.4(3) 1_665 8_666 ?
O11 Na1 O11 180.0 7_556 1_665 ?
O12 Na1 O12 140.1(10) 7_556 8_666 ?
O12 Na1 O12 180.0 8_666 2 ?
O12 Na1 O12 180.0 7_556 1_665 ?
O12 Na1 O12 39.9(10) 1_665 8_666 ?
O12 Na1 O12 39.9(10) 7_556 2 ?
O12 Na1 O12 140.1(10) 1_665 2 ?
Na3 Na3 Na3 60.0 3_565 2_665 ?
F2 Na3 Na3 46.90(5) . 2_665 ?
F2 Na3 Na3 46.90(5) . 3_565 ?
F2 Na3 O2 115.96(13) . . ?
F2 Na3 O9 147.85(13) . 3_665 ?
F2 Na3 O4 84.01(16) . . ?
F2 Na3 O4 84.01(16) . 3_565 ?
F2 Na3 O5 73.41(19) . 3_565 ?
F2 Na3 O5 73.41(19) . . ?
F2 Na3 O8 153.7(6) . . ?
F2 Na3 O8 153.7(6) . 3_665 ?
F3 Na3 Na3 46.52(6) . 2_665 ?
F3 Na3 Na3 46.52(6) . 3_565 ?
F3 Na3 F2 75.30(11) . . ?
F3 Na3 O2 168.74(15) . . ?
F3 Na3 O9 72.56(13) . 3_665 ?
F3 Na3 O4 76.65(15) . 3_565 ?
F3 Na3 O4 76.65(15) . . ?
F3 Na3 O5 86.8(2) . 3_565 ?
F3 Na3 O5 86.8(2) . . ?
F3 Na3 O8 90.9(6) . . ?
F3 Na3 O8 90.9(6) . 3_665 ?
O2 Na3 Na3 141.03(7) . 3_565 ?
O2 Na3 Na3 141.03(7) . 2_665 ?
O2 Na3 O8 78.7(6) . 3_665 ?
O2 Na3 O8 78.7(6) . . ?
O9 Na3 Na3 107.18(8) 3_665 2_665 ?
O9 Na3 Na3 107.18(9) 3_665 3_565 ?
O9 Na3 O2 96.19(15) 3_665 . ?
O4 Na3 Na3 47.95(14) 3_565 3_565 ?
O4 Na3 Na3 47.96(14) . 2_665 ?
O4 Na3 Na3 107.58(14) 3_565 2_665 ?
O4 Na3 Na3 107.58(14) . 3_565 ?
O4 Na3 O2 103.63(14) 3_565 . ?
O4 Na3 O2 103.63(14) . . ?
O4 Na3 O9 88.62(17) 3_565 3_665 ?
O4 Na3 O9 88.62(17) . 3_665 ?
O4 Na3 O4 152.7(3) 3_565 . ?
O5 Na3 Na3 107.07(16) 3_565 2_665 ?
O5 Na3 Na3 107.07(16) . 3_565 ?
O5 Na3 Na3 48.34(16) . 2_665 ?
O5 Na3 Na3 48.34(16) 3_565 3_565 ?
O5 Na3 O2 96.25(19) 3_565 . ?
O5 Na3 O2 96.25(19) . . ?
O5 Na3 O5 146.8(4) . 3_565 ?
O5 Na3 O8 129.0(6) 3_565 3_665 ?
O5 Na3 O8 83.7(6) 3_565 . ?
O5 Na3 O8 83.7(6) . 3_665 ?
O5 Na3 O8 129.0(6) . . ?
O8 Na3 Na3 107.6(6) 3_665 2_665 ?
O8 Na3 Na3 107.6(6) . 3_565 ?
O8 Na3 Na3 133.5(5) . 2_665 ?
O8 Na3 Na3 133.5(5) 3_665 3_565 ?
O8 Na3 O8 45.4(11) . 3_665 ?
Na2 Na2 Na2 60.0 2_665 3_565 ?
F2 Na2 Na2 45.83(6) . 2_665 ?
F2 Na2 Na2 45.83(6) . 3_565 ?
F2 Na2 F1 77.84(10) . . ?
F2 Na2 O1 82.98(7) . 3_565 ?
F2 Na2 O1 82.98(7) . . ?
F2 Na2 O11 145.5(2) . 7_556 ?
F2 Na2 O5 72.9(2) . 3_565 ?
F2 Na2 O6 117.3(3) . 1_445 ?
F2 Na2 O10 169.7(2) . . ?
F2 Na2 O12 152.1(5) . 3 ?
F2 Na2 O12 152.1(5) . 2 ?
F1 Na2 Na2 49.49(6) . 3_565 ?
F1 Na2 Na2 49.49(6) . 2_665 ?
F1 Na2 O11 67.7(2) . 7_556 ?
F1 Na2 O5 150.8(3) . 3_565 ?
F1 Na2 O12 86.6(6) . 2 ?
F1 Na2 O12 86.6(6) . 3 ?
O1 Na2 Na2 47.82(6) . 2_665 ?
O1 Na2 Na2 47.81(6) 3_565 3_565 ?
O1 Na2 Na2 107.57(6) 3_565 2_665 ?
O1 Na2 Na2 107.57(6) . 3_565 ?
O1 Na2 F1 77.57(7) 3_565 . ?
O1 Na2 F1 77.57(7) . . ?
O1 Na2 O1 153.51(12) 3_565 . ?
O1 Na2 O11 89.47(9) 3_565 7_556 ?
O1 Na2 O11 89.48(9) . 7_556 ?
O1 Na2 O5 98.60(9) . 3_565 ?
O1 Na2 O5 98.60(9) 3_565 3_565 ?
O1 Na2 O6 103.20(6) . 1_445 ?
O1 Na2 O6 103.20(6) 3_565 1_445 ?
O1 Na2 O10 98.91(8) 3_565 . ?
O1 Na2 O10 98.92(8) . . ?
O1 Na2 O12 71.0(4) . 2 ?
O1 Na2 O12 116.3(4) 3_565 2 ?
O1 Na2 O12 116.3(4) . 3 ?
O1 Na2 O12 71.0(4) 3_565 3 ?
O11 Na2 Na2 106.43(18) 7_556 2_665 ?
O11 Na2 Na2 106.43(18) 7_556 3_565 ?
O5 Na2 Na2 106.7(2) 3_565 2_665 ?
O5 Na2 Na2 106.7(2) 3_565 3_565 ?
O5 Na2 O12 120.0(6) 3_565 2 ?
O5 Na2 O12 120.0(6) 3_565 3 ?
O6 Na2 Na2 140.93(15) 1_445 2_665 ?
O6 Na2 Na2 140.93(15) 1_445 3_565 ?
O6 Na2 F1 164.9(3) 1_445 . ?
O6 Na2 O5 44.3(4) 1_445 3_565 ?
O6 Na2 O12 79.5(6) 1_445 3 ?
O6 Na2 O12 79.5(6) 1_445 2 ?
O10 Na2 Na2 141.06(13) . 2_665 ?
O10 Na2 Na2 141.06(13) . 3_565 ?
O10 Na2 F1 112.5(2) . . ?
O10 Na2 O11 44.8(3) . 7_556 ?
O10 Na2 O5 96.7(3) . 3_565 ?
O10 Na2 O6 52.4(4) . 1_445 ?
O10 Na2 O12 34.5(6) . 2 ?
O10 Na2 O12 34.5(6) . 3 ?
O12 Na2 Na2 133.1(5) 2 3_565 ?
O12 Na2 Na2 133.1(5) 3 2_665 ?
O12 Na2 Na2 106.8(5) 2 2_665 ?
O12 Na2 Na2 106.8(5) 3 3_565 ?
O12 Na2 O12 46.5(7) 3 2 ?
Cl1 Na4 Na3 135.46(6) . . ?
Cl1 Na4 Na4 134.52(3) . 2_665 ?
Cl1 Na4 Na4 134.52(3) . 3_565 ?
Na4 Na4 Na3 60.56(4) 2_665 . ?
Na4 Na4 Na3 90.02(4) 3_565 . ?
Na4 Na4 Na4 60.000(1) 3_565 2_665 ?
F3 Na4 Cl1 178.51(12) . . ?
F3 Na4 Na3 45.62(7) . . ?
F3 Na4 Na4 44.43(7) . 2_665 ?
F3 Na4 Na4 44.43(7) . 3_565 ?
F3 Na4 O7 76.48(14) . 7_665 ?
F3 Na4 O9 74.47(9) . 3_665 ?
F3 Na4 O9 74.47(9) . 2 ?
F3 Na4 O4 74.5(2) . 3_565 ?
F3 Na4 O3 115.0(3) . 1_445 ?
F3 Na4 O8 95.4(6) . . ?
F3 Na4 O8 95.4(6) . 2 ?
O7 Na4 Cl1 102.03(12) 7_665 . ?
O7 Na4 Na3 109.91(10) 7_665 . ?
O7 Na4 Na4 49.96(8) 7_665 2_665 ?
O7 Na4 Na4 49.96(8) 7_665 3_565 ?
O7 Na4 O4 151.0(2) 7_665 3_565 ?
O7 Na4 O3 168.6(2) 7_665 1_445 ?
O7 Na4 O8 113.2(5) 7_665 . ?
O7 Na4 O8 113.2(5) 7_665 2 ?
O9 Na4 Cl1 105.55(9) 2 . ?
O9 Na4 Cl1 105.55(9) 3_665 . ?
O9 Na4 Na3 47.96(10) 3_665 . ?
O9 Na4 Na3 106.14(12) 2 . ?
O9 Na4 Na4 107.37(8) 3_665 3_565 ?
O9 Na4 Na4 48.33(8) 3_665 2_665 ?
O9 Na4 Na4 107.37(8) 2 2_665 ?
O9 Na4 Na4 48.33(8) 2 3_565 ?
O9 Na4 O7 87.33(10) 3_665 7_665 ?
O9 Na4 O7 87.33(10) 2 7_665 ?
O9 Na4 O9 148.88(18) 3_665 2 ?
O9 Na4 O4 84.98(12) 2 3_565 ?
O9 Na4 O4 84.98(12) 3_665 3_565 ?
O9 Na4 O3 95.63(11) 3_665 1_445 ?
O9 Na4 O3 95.63(11) 2 1_445 ?
O4 Na4 Cl1 107.0(2) 3_565 . ?
O4 Na4 Na3 46.63(14) 3_565 . ?
O4 Na4 Na4 106.32(16) 3_565 2_665 ?
O4 Na4 Na4 106.32(16) 3_565 3_565 ?
O3 Na4 Cl1 66.5(2) 1_445 . ?
O3 Na4 Na3 79.9(2) 1_445 . ?
O3 Na4 Na4 138.21(15) 1_445 3_565 ?
O3 Na4 Na4 138.21(15) 1_445 2_665 ?
O3 Na4 O4 40.5(3) 1_445 3_565 ?
O8 Na4 Cl1 85.1(6) 2 . ?
O8 Na4 Cl1 85.1(6) . . ?
O8 Na4 Na3 54.3(7) . . ?
O8 Na4 Na3 108.6(7) 2 . ?
O8 Na4 Na4 135.6(5) 2 2_665 ?
O8 Na4 Na4 135.6(5) . 3_565 ?
O8 Na4 Na4 78.2(5) 2 3_565 ?
O8 Na4 Na4 78.2(5) . 2_665 ?
O8 Na4 O8 133.5(10) . 2 ?
Na3 F2 Na3 86.20(10) 3_565 . ?
Na3 F2 Na3 86.20(10) 3_565 2_665 ?
Na3 F2 Na3 86.20(10) 2_665 . ?
Na2 F2 Na3 92.72(5) . 3_565 ?
Na2 F2 Na3 178.52(14) . 2_665 ?
Na2 F2 Na3 92.72(5) . . ?
Na2 F2 Na3 178.52(14) 2_665 3_565 ?
Na2 F2 Na3 178.52(14) 3_565 . ?
Na2 F2 Na3 92.72(5) 3_565 3_565 ?
Na2 F2 Na3 92.72(5) 3_565 2_665 ?
Na2 F2 Na3 92.72(5) 2_665 2_665 ?
Na2 F2 Na3 92.72(5) 2_665 . ?
Na2 F2 Na2 88.33(11) 3_565 2_665 ?
Na2 F2 Na2 88.33(11) 3_565 . ?
Na2 F2 Na2 88.33(11) . 2_665 ?
Na1 F1 Na1 102.01(11) 3_565 . ?
Na1 F1 Na1 102.01(11) 2_665 3_565 ?
Na1 F1 Na1 102.01(11) 2_665 . ?
Na1 F1 Na2 164.77(16) . 3_565 ?
Na1 F1 Na2 87.43(3) . . ?
Na1 F1 Na2 87.43(3) 2_665 3_565 ?
Na1 F1 Na2 164.77(16) 3_565 2_665 ?
Na1 F1 Na2 87.43(3) . 2_665 ?
Na1 F1 Na2 87.43(3) 2_665 2_665 ?
Na1 F1 Na2 164.77(16) 2_665 . ?
Na1 F1 Na2 87.43(3) 3_565 . ?
Na1 F1 Na2 87.43(3) 3_565 3_565 ?
Na2 F1 Na2 81.02(12) 2_665 . ?
Na2 F1 Na2 81.02(12) 3_565 2_665 ?
Na2 F1 Na2 81.02(12) 3_565 . ?
Na3 F3 Na3 86.96(12) 3_565 . ?
Na3 F3 Na3 86.96(12) 2_665 . ?
Na3 F3 Na3 86.96(12) 2_665 3_565 ?
Na4 F3 Na3 177.06(17) . 2_665 ?
Na4 F3 Na3 90.91(5) 2_665 2_665 ?
Na4 F3 Na3 90.91(5) . . ?
Na4 F3 Na3 90.91(5) 3_565 2_665 ?
Na4 F3 Na3 177.06(17) 3_565 . ?
Na4 F3 Na3 177.06(17) 2_665 3_565 ?
Na4 F3 Na3 90.91(5) . 3_565 ?
Na4 F3 Na3 90.91(5) 2_665 . ?
Na4 F3 Na3 90.91(5) 3_565 3_565 ?
Na4 F3 Na4 91.15(13) . 2_665 ?
Na4 F3 Na4 91.15(13) 3_565 2_665 ?
Na4 F3 Na4 91.15(13) 3_565 . ?
S1 O1 Na1 124.62(18) . . ?
S1 O1 Na2 131.78(10) . 2_665 ?
S1 O1 Na2 131.78(10) . . ?
Na2 O1 Na1 83.59(9) . . ?
Na2 O1 Na1 83.59(9) 2_665 . ?
Na2 O1 Na2 84.37(12) 2_665 . ?
S1 O2 Na3 116.13(11) . . ?
S1 O2 Na3 116.13(11) . 3_665 ?
S1 O2 Na3 116.13(11) . 2_655 ?
Na3 O2 Na3 102.07(13) 3_665 . ?
Na3 O2 Na3 102.07(13) 2_655 3_665 ?
Na3 O2 Na3 102.07(13) 2_655 . ?
S3 O7 Na4 132.03(11) . 9_655 ?
S3 O7 Na4 132.03(11) . 8 ?
S3 O7 Na4 132.03(11) . 7_665 ?
Na4 O7 Na4 80.08(16) 9_655 7_665 ?
Na4 O7 Na4 80.08(16) 9_655 8 ?
Na4 O7 Na4 80.08(16) 8 7_665 ?
S3 O9 Na3 129.9(3) . 2_655 ?
S3 O9 Na4 128.93(15) . 2_655 ?
S3 O9 Na4 128.93(15) . 3 ?
Na4 O9 Na3 84.65(12) 3 2_655 ?
Na4 O9 Na3 84.65(12) 2_655 2_655 ?
Na4 O9 Na4 83.33(15) 2_655 3 ?
S4 O11 Na1 130.7(2) . 1_445 ?
S4 O11 Na1 130.7(2) . 3 ?
S4 O11 Na2 119.6(6) . 7_556 ?
S4 O11 O11 58.37(15) . 8_556 ?
S4 O11 O11 58.37(15) . 9_556 ?
Na1 O11 Na1 92.6(3) 1_445 3 ?
Na1 O11 Na2 83.0(2) 1_445 7_556 ?
Na1 O11 Na2 83.0(2) 3 7_556 ?
O11 O11 Na1 150.4(10) 8_556 3 ?
O11 O11 Na1 72.30(15) 8_556 1_445 ?
O11 O11 Na1 150.4(10) 9_556 1_445 ?
O11 O11 Na1 72.30(15) 9_556 3 ?
O11 O11 Na2 118.9(9) 9_556 7_556 ?
O11 O11 Na2 118.9(9) 8_556 7_556 ?
O11 O11 O11 108.5(9) 9_556 8_556 ?
S2 O4 Na3 132.3(2) . 2_665 ?
S2 O4 Na3 132.3(2) . . ?
S2 O4 Na4 126.1(5) . 2_665 ?
S2 O4 O3 57.4(4) . . ?
Na3 O4 Na3 84.1(3) 2_665 . ?
Na3 O4 Na4 81.9(2) 2_665 2_665 ?
Na3 O4 Na4 81.9(2) . 2_665 ?
O3 O4 Na3 128.9(3) . . ?
O3 O4 Na3 128.9(3) . 2_665 ?
O3 O4 Na4 68.7(4) . 2_665 ?
S2 O5 Na3 132.0(3) . 2_665 ?
S2 O5 Na3 132.0(3) . . ?
S2 O5 Na2 121.2(6) . 2_665 ?
Na3 O5 Na3 83.3(3) 2_665 . ?
Na3 O5 Na2 86.5(3) . 2_665 ?
Na3 O5 Na2 86.5(3) 2_665 2_665 ?
S2 O6 Na2 116.3(3) . 3_665 ?
S2 O6 Na2 116.3(3) . 1_665 ?
S2 O6 Na2 116.3(3) . 2_665 ?
Na2 O6 Na2 101.9(3) 3_665 2_665 ?
Na2 O6 Na2 101.9(3) 3_665 1_665 ?
Na2 O6 Na2 101.9(3) 1_665 2_665 ?
S2 O3 Na4 120.6(2) . 2_665 ?
S2 O3 Na4 120.6(2) . 1_665 ?
S2 O3 Na4 120.6(2) . 3_665 ?
S2 O3 O4 49.7(4) . . ?
S2 O3 O4 49.7(4) . 2_765 ?
S2 O3 O4 49.7(4) . 3_675 ?
Na4 O3 Na4 96.4(3) 2_665 3_665 ?
Na4 O3 Na4 96.4(3) 2_665 1_665 ?
Na4 O3 Na4 96.4(3) 1_665 3_665 ?
O4 O3 Na4 131.10(8) . 3_665 ?
O4 O3 Na4 131.10(8) . 1_665 ?
O4 O3 Na4 131.10(8) 3_675 3_665 ?
O4 O3 Na4 131.10(8) 3_675 2_665 ?
O4 O3 Na4 131.10(8) 2_765 2_665 ?
O4 O3 Na4 70.9(2) . 2_665 ?
O4 O3 Na4 131.10(8) 2_765 1_665 ?
O4 O3 Na4 70.9(2) 2_765 3_665 ?
O4 O3 Na4 70.9(2) 3_675 1_665 ?
O4 O3 O4 82.7(6) 3_675 2_765 ?
O4 O3 O4 82.7(6) 2_765 . ?
O4 O3 O4 82.7(6) 3_675 . ?
S4 O10 Na2 116.1(2) . . ?
S4 O10 Na2 116.1(2) . 2 ?
S4 O10 Na2 116.1(2) . 3 ?
S4 O10 O12 53.2(10) . 2 ?
S4 O10 O12 53.2(10) . . ?
S4 O10 O12 53.2(10) . 3 ?
Na2 O10 Na2 102.1(3) 3 2 ?
Na2 O10 Na2 102.1(3) 3 . ?
Na2 O10 Na2 102.1(3) . 2 ?
O12 O10 Na2 169.3(11) 3 3 ?
O12 O10 Na2 169.3(11) 2 2 ?
O12 O10 Na2 84.5(6) . 2 ?
O12 O10 Na2 84.5(6) 2 3 ?
O12 O10 Na2 84.5(6) 2 . ?
O12 O10 Na2 169.3(11) . . ?
O12 O10 Na2 84.5(6) . 3 ?
O12 O10 Na2 84.5(6) 3 2 ?
O12 O10 Na2 84.5(6) 3 . ?
O12 O10 O12 87.9(14) . 2 ?
O12 O10 O12 87.9(14) 2 3 ?
O12 O10 O12 87.9(14) . 3 ?
S3 O8 Na3 110.6(13) . 2_655 ?
S3 O8 Na3 110.6(13) . . ?
S3 O8 Na4 113.8(12) . . ?
S3 O8 Na4 113.8(12) . 3 ?
Na3 O8 Na3 87.1(10) 2_655 . ?
Na4 O8 Na3 135.5(10) 3 . ?
Na4 O8 Na3 135.5(10) . 2_655 ?
Na4 O8 Na3 74.2(3) 3 2_655 ?
Na4 O8 Na3 74.2(3) . . ?
Na4 O8 Na4 91.2(10) . 3 ?
S4 O12 Na1 121.6(13) . 3 ?
S4 O12 Na1 121.6(13) . 1_445 ?
S4 O12 Na2 104.8(13) . 3 ?
S4 O12 Na2 104.8(13) . 2 ?
S4 O12 O10 62.0(11) . . ?
S4 O12 O12 51.5(10) . 8_556 ?
S4 O12 O12 51.5(10) . 9_556 ?
Na1 O12 Na1 86.4(9) 1_445 3 ?
Na1 O12 Na2 75.2(3) 1_445 2 ?
Na1 O12 Na2 75.2(3) 3 3 ?
Na1 O12 Na2 132.9(8) 3 2 ?
Na1 O12 Na2 132.9(8) 1_445 3 ?
Na2 O12 Na2 86.3(11) 2 3 ?
O10 O12 Na1 133.9(9) . 1_445 ?
O10 O12 Na1 133.9(9) . 3 ?
O10 O12 Na2 61.1(10) . 3 ?
O10 O12 Na2 61.1(10) . 2 ?
O10 O12 O12 96.9(11) . 8_556 ?
O10 O12 O12 96.9(11) . 9_556 ?
O12 O12 Na1 70.1(5) 8_556 1_445 ?
O12 O12 Na1 121(3) 8_556 3 ?
O12 O12 Na1 70.1(5) 9_556 3 ?
O12 O12 Na1 121(3) 9_556 1_445 ?
O12 O12 Na2 155.2(10) 8_556 3 ?
O12 O12 Na2 92.7(16) 9_556 3 ?
O12 O12 Na2 155.2(10) 9_556 2 ?
O12 O12 Na2 92.7(16) 8_556 2 ?
O12 O12 O12 78(3) 9_556 8_556 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
S1 Na3 3.3721(19) 2_655 ?
S1 Na3 3.3721(19) . ?
S1 Na3 3.3721(19) 3_665 ?
S1 O1 1.464(3) . ?
S1 O1 1.464(3) 2_655 ?
S1 O1 1.464(3) 3_665 ?
S1 O2 1.462(5) . ?
S4 O11 1.417(8) . ?
S4 O11 1.417(8) 7_556 ?
S4 O11 1.417(8) 8_556 ?
S4 O11 1.417(8) 2 ?
S4 O11 1.417(8) 9_556 ?
S4 O11 1.417(8) 3 ?
S4 O12 1.416(19) 7_556 ?
S4 O12 1.416(19) . ?
S4 O12 1.416(19) 8_556 ?
S4 O12 1.416(19) 2 ?
S4 O12 1.416(19) 9_556 ?
S4 O12 1.416(19) 3 ?
S3 O7 1.425(6) . ?
S3 O9 1.460(4) 2_655 ?
S3 O9 1.460(4) . ?
S3 O9 1.460(4) 3_665 ?
S3 O8 1.47(3) 3_665 ?
S3 O8 1.47(3) . ?
S3 O8 1.47(3) 2_655 ?
S2 O4 1.430(8) 3_675 ?
S2 O4 1.430(8) 2_765 ?
S2 O4 1.430(8) . ?
S2 O5 1.414(9) 2_765 ?
S2 O5 1.414(9) 3_675 ?
S2 O5 1.414(9) . ?
S2 O6 1.565(12) . ?
S2 O3 1.579(12) . ?
Cl1 Na4 2.732(2) 8 ?
Cl1 Na4 2.732(2) 2 ?
Cl1 Na4 2.732(2) 9 ?
Cl1 Na4 2.732(2) 7 ?
Cl1 Na4 2.732(2) 3 ?
Cl1 Na4 2.732(2) . ?
Na1 F1 2.2746(18) . ?
Na1 F1 2.2746(18) 7_666 ?
Na1 O1 2.534(3) 7_666 ?
Na1 O1 2.534(3) . ?
Na1 O11 2.445(6) 8_666 ?
Na1 O11 2.445(6) 7_556 ?
Na1 O11 2.445(6) 1_665 ?
Na1 O11 2.445(6) 2 ?
Na1 O12 2.58(2) 7_556 ?
Na1 O12 2.58(2) 2 ?
Na1 O12 2.58(2) 8_666 ?
Na1 O12 2.58(2) 1_665 ?
Na3 Na3 3.242(3) 3_565 ?
Na3 Na3 3.242(3) 2_665 ?
Na3 F2 2.373(3) . ?
Na3 F3 2.356(3) . ?
Na3 O2 2.462(3) . ?
Na3 O9 2.459(4) 3_665 ?
Na3 O4 2.421(6) 3_565 ?
Na3 O4 2.421(6) . ?
Na3 O5 2.439(8) . ?
Na3 O5 2.439(8) 3_565 ?
Na3 O8 2.78(2) . ?
Na3 O8 2.78(2) 3_665 ?
Na2 Na2 3.229(3) 2_665 ?
Na2 Na2 3.229(3) 3_565 ?
Na2 F2 2.317(3) . ?
Na2 F1 2.486(3) . ?
Na2 O1 2.405(2) 3_565 ?
Na2 O1 2.405(2) . ?
Na2 O11 2.527(11) 7_556 ?
Na2 O5 2.515(10) 3_565 ?
Na2 O6 2.474(6) 1_445 ?
Na2 O10 2.470(5) . ?
Na2 O12 2.81(3) 2 ?
Na2 O12 2.81(3) 3 ?
Na4 Na4 3.240(3) 2_665 ?
Na4 Na4 3.240(3) 3_565 ?
Na4 F3 2.268(3) . ?
Na4 O7 2.518(4) 7_665 ?
Na4 O9 2.437(3) 2 ?
Na4 O9 2.437(3) 3_665 ?
Na4 O4 2.606(7) 3_565 ?
Na4 O3 2.570(6) 1_445 ?
Na4 O8 2.68(2) . ?
Na4 O8 2.68(2) 2 ?
F2 Na3 2.373(3) 2_665 ?
F2 Na3 2.373(3) 3_565 ?
F2 Na2 2.318(3) 3_565 ?
F2 Na2 2.317(3) 2_665 ?
F1 Na1 2.2746(18) 3_565 ?
F1 Na1 2.2746(18) 2_665 ?
F1 Na2 2.486(3) 2_665 ?
F1 Na2 2.486(3) 3_565 ?
F3 Na3 2.356(3) 3_565 ?
F3 Na3 2.356(3) 2_665 ?
F3 Na4 2.268(3) 3_565 ?
F3 Na4 2.268(3) 2_665 ?
O1 Na2 2.405(2) 2_665 ?
O2 Na3 2.462(3) 2_655 ?
O2 Na3 2.462(3) 3_665 ?
O7 Na4 2.518(4) 8 ?
O7 Na4 2.518(4) 9_655 ?
O7 Na4 2.518(4) 7_665 ?
O9 Na3 2.459(4) 2_655 ?
O9 Na4 2.437(3) 3 ?
O9 Na4 2.437(3) 2_655 ?
O11 Na1 2.445(6) 1_445 ?
O11 Na1 2.445(6) 3 ?
O11 Na2 2.527(11) 7_556 ?
O11 O11 1.486(10) 9_556 ?
O11 O11 1.486(10) 8_556 ?
O4 Na3 2.421(6) 2_665 ?
O4 Na4 2.606(7) 2_665 ?
O4 O3 1.791(11) . ?
O5 Na3 2.439(8) 2_665 ?
O5 Na2 2.515(10) 2_665 ?
O6 Na2 2.474(6) 3_665 ?
O6 Na2 2.474(6) 2_665 ?
O6 Na2 2.474(6) 1_665 ?
O3 Na4 2.570(6) 1_665 ?
O3 Na4 2.570(6) 3_665 ?
O3 Na4 2.570(6) 2_665 ?
O3 O4 1.791(11) 3_675 ?
O3 O4 1.791(11) 2_765 ?
O10 Na2 2.470(5) 3 ?
O10 Na2 2.470(5) 2 ?
O10 O12 1.60(4) 3 ?
O10 O12 1.60(4) 2 ?
O10 O12 1.60(4) . ?
O8 Na3 2.78(2) 2_655 ?
O8 Na4 2.68(2) 3 ?
O12 Na1 2.58(2) 1_445 ?
O12 Na1 2.58(2) 3 ?
O12 Na2 2.81(3) 2 ?
O12 Na2 2.81(3) 3 ?
O12 O12 1.76(5) 8_556 ?
O12 O12 1.76(5) 9_556 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
S4 O10 O12 Na1 108.2(17) . . . 1_445 ?
S4 O10 O12 Na1 -108.2(17) . . . 3 ?
S4 O10 O12 Na2 128.61(15) . . . 2 ?
S4 O10 O12 Na2 -128.61(15) . . . 3 ?
S4 O10 O12 O12 -39.3(15) . . . 9_556 ?
S4 O10 O12 O12 39.3(15) . . . 8_556 ?
S2 O4 O3 Na4 -98.4(6) . . . 1_665 ?
S2 O4 O3 Na4 98.4(6) . . . 3_665 ?
S2 O4 O3 Na4 179.999(0) . . . 2_665 ?
S2 O4 O3 O4 -41.8(2) . . . 3_675 ?
S2 O4 O3 O4 41.8(2) . . . 2_765 ?
Na3 S1 O1 Na1 136.70(8) 2_655 . . . ?
Na3 S1 O1 Na1 180.000(0) . . . . ?
Na3 S1 O1 Na1 -136.70(8) 3_665 . . . ?
Na3 S1 O1 Na2 20.9(3) 2_655 . . . ?
Na3 S1 O1 Na2 64.2(2) . . . . ?
Na3 S1 O1 Na2 -107.52(15) 2_655 . . 2_665 ?
Na3 S1 O1 Na2 -20.9(3) 3_665 . . 2_665 ?
Na3 S1 O1 Na2 107.52(15) 3_665 . . . ?
Na3 S1 O1 Na2 -64.2(2) . . . 2_665 ?
Na3 S1 O2 Na3 -120.001(1) . . . 2_655 ?
Na3 S1 O2 Na3 119.999(0) 3_665 . . 2_655 ?
Na3 S1 O2 Na3 120.001(1) . . . 3_665 ?
Na3 S1 O2 Na3 -119.999(0) 2_655 . . 3_665 ?
Na3 S1 O2 Na3 -120.001(1) 3_665 . . . ?
Na3 S1 O2 Na3 120.001(1) 2_655 . . . ?
Na3 O4 O3 S2 -120.7(4) . . . . ?
Na3 O4 O3 S2 120.7(4) 2_665 . . . ?
Na3 O4 O3 Na4 22.3(9) 2_665 . . 1_665 ?
Na3 O4 O3 Na4 -59.3(4) 2_665 . . 2_665 ?
Na3 O4 O3 Na4 -140.9(4) 2_665 . . 3_665 ?
Na3 O4 O3 Na4 140.9(4) . . . 1_665 ?
Na3 O4 O3 Na4 59.3(4) . . . 2_665 ?
Na3 O4 O3 Na4 -22.3(9) . . . 3_665 ?
Na3 O4 O3 O4 78.9(6) 2_665 . . 3_675 ?
Na3 O4 O3 O4 -162.4(2) . . . 3_675 ?
Na3 O4 O3 O4 -78.9(6) . . . 2_765 ?
Na3 O4 O3 O4 162.4(2) 2_665 . . 2_765 ?
Na2 O10 O12 S4 128.61(15) 3 . . . ?
Na2 O10 O12 S4 -128.61(15) 2 . . . ?
Na2 O10 O12 S4 0.000(19) . . . . ?
Na2 O10 O12 Na1 123.2(17) 2 . . 3 ?
Na2 O10 O12 Na1 -20.4(16) 2 . . 1_445 ?
Na2 O10 O12 Na1 -123.2(17) 3 . . 1_445 ?
Na2 O10 O12 Na1 20.4(16) 3 . . 3 ?
Na2 O10 O12 Na1 108.2(17) . . . 1_445 ?
Na2 O10 O12 Na1 -108.2(17) . . . 3 ?
Na2 O10 O12 Na2 -102.8(3) 3 . . 2 ?
Na2 O10 O12 Na2 102.8(3) 2 . . 3 ?
Na2 O10 O12 Na2 128.61(16) . . . 2 ?
Na2 O10 O12 Na2 -128.61(16) . . . 3 ?
Na2 O10 O12 O12 168.0(16) 3 . . 8_556 ?
Na2 O10 O12 O12 39.3(16) . . . 8_556 ?
Na2 O10 O12 O12 -89.3(15) 2 . . 8_556 ?
Na2 O10 O12 O12 -168.0(16) 2 . . 9_556 ?
Na2 O10 O12 O12 89.3(15) 3 . . 9_556 ?
Na2 O10 O12 O12 -39.3(15) . . . 9_556 ?
Na4 O4 O3 S2 180.001(0) 2_665 . . . ?
Na4 O4 O3 Na4 81.6(6) 2_665 . . 1_665 ?
Na4 O4 O3 Na4 -81.6(6) 2_665 . . 3_665 ?
Na4 O4 O3 O4 138.2(2) 2_665 . . 3_675 ?
Na4 O4 O3 O4 -138.2(2) 2_665 . . 2_765 ?
O1 S1 O1 Na1 -59.98(16) 3_665 . . . ?
O1 S1 O1 Na1 59.98(16) 2_655 . . . ?
O1 S1 O1 Na2 175.75(7) 2_655 . . 2_665 ?
O1 S1 O1 Na2 -55.8(4) 2_655 . . . ?
O1 S1 O1 Na2 -175.75(7) 3_665 . . . ?
O1 S1 O1 Na2 55.8(4) 3_665 . . 2_665 ?
O1 S1 O2 Na3 0.001(0) 3_665 . . 3_665 ?
O1 S1 O2 Na3 120.000(0) 2_655 . . . ?
O1 S1 O2 Na3 -120.001(1) . . . 2_655 ?
O1 S1 O2 Na3 -120.000(0) 3_665 . . . ?
O1 S1 O2 Na3 0.000(0) . . . . ?
O1 S1 O2 Na3 119.999(1) 3_665 . . 2_655 ?
O1 S1 O2 Na3 -0.001(1) 2_655 . . 2_655 ?
O1 S1 O2 Na3 120.001(0) . . . 3_665 ?
O1 S1 O2 Na3 -119.999(1) 2_655 . . 3_665 ?
O2 S1 O1 Na1 180.000(0) . . . . ?
O2 S1 O1 Na2 64.2(2) . . . . ?
O2 S1 O1 Na2 -64.2(2) . . . 2_665 ?
O7 S3 O9 Na3 179.999(0) . . . 2_655 ?
O7 S3 O9 Na4 58.7(2) . . . 2_655 ?
O7 S3 O9 Na4 -58.7(2) . . . 3 ?
O7 S3 O8 Na3 -132.6(10) . . . . ?
O7 S3 O8 Na3 132.6(10) . . . 2_655 ?
O7 S3 O8 Na4 51.3(12) . . . 3 ?
O7 S3 O8 Na4 -51.3(12) . . . . ?
O9 S3 O7 Na4 -60.000(1) 2_655 . . 7_665 ?
O9 S3 O7 Na4 180.0 . . . 7_665 ?
O9 S3 O7 Na4 60.000(0) 2_655 . . 9_655 ?
O9 S3 O7 Na4 60.001(1) . . . 8 ?
O9 S3 O7 Na4 -60.000(0) . . . 9_655 ?
O9 S3 O7 Na4 180.001(1) 2_655 . . 8 ?
O9 S3 O7 Na4 180.000(0) 3_665 . . 9_655 ?
O9 S3 O7 Na4 60.000(0) 3_665 . . 7_665 ?
O9 S3 O7 Na4 -59.999(1) 3_665 . . 8 ?
O9 S3 O9 Na3 -59.4(2) 3_665 . . 2_655 ?
O9 S3 O9 Na3 59.4(2) 2_655 . . 2_655 ?
O9 S3 O9 Na4 -61.9(5) 2_655 . . 2_655 ?
O9 S3 O9 Na4 61.9(5) 3_665 . . 3 ?
O9 S3 O9 Na4 -179.31(7) 2_655 . . 3 ?
O9 S3 O9 Na4 179.32(7) 3_665 . . 2_655 ?
O11 S4 O11 Na1 0.000(1) 8_556 . . 1_445 ?
O11 S4 O11 Na1 180.000(1) 3 . . 3 ?
O11 S4 O11 Na1 144.8(15) 8_556 . . 3 ?
O11 S4 O11 Na1 180.000(1) 2 . . 1_445 ?
O11 S4 O11 Na1 -144.8(15) 9_556 . . 1_445 ?
O11 S4 O11 Na1 0.000(1) 9_556 . . 3 ?
O11 S4 O11 Na1 -35.2(15) 2 . . 3 ?
O11 S4 O11 Na1 35.2(15) 3 . . 1_445 ?
O11 S4 O11 Na2 72.4(7) 2 . . 7_556 ?
O11 S4 O11 Na2 -107.6(7) 8_556 . . 7_556 ?
O11 S4 O11 Na2 -72.4(7) 3 . . 7_556 ?
O11 S4 O11 Na2 107.6(7) 9_556 . . 7_556 ?
O11 S4 O11 O11 144.8(15) 8_556 . . 9_556 ?
O11 S4 O11 O11 180.000(0) 2 . . 8_556 ?
O11 S4 O11 O11 180.000(2) 3 . . 9_556 ?
O11 S4 O11 O11 -144.8(15) 9_556 . . 8_556 ?
O11 S4 O11 O11 35.2(15) 3 . . 8_556 ?
O11 S4 O11 O11 -35.2(15) 2 . . 9_556 ?
O11 S4 O10 Na2 -60.000(1) . . . 3 ?
O11 S4 O10 Na2 -59.999(0) 3 . . 2 ?
O11 S4 O10 Na2 180.000(1) 3 . . 3 ?
O11 S4 O10 Na2 0.001(0) 8_556 . . 2 ?
O11 S4 O10 Na2 -120.000(0) 9_556 . . . ?
O11 S4 O10 Na2 -60.000(0) 2 . . . ?
O11 S4 O10 Na2 60.000(0) 3 . . . ?
O11 S4 O10 Na2 -120.000(1) 8_556 . . 3 ?
O11 S4 O10 Na2 120.000(0) 8_556 . . . ?
O11 S4 O10 Na2 0.000(1) 9_556 . . 3 ?
O11 S4 O10 Na2 120.001(1) 9_556 . . 2 ?
O11 S4 O10 Na2 60.000(1) 2 . . 3 ?
O11 S4 O10 Na2 -119.999(0) 7_556 . . 2 ?
O11 S4 O10 Na2 120.000(1) 7_556 . . 3 ?
O11 S4 O10 Na2 180.000(0) . . . . ?
O11 S4 O10 Na2 60.001(0) . . . 2 ?
O11 S4 O10 Na2 0.000(0) 7_556 . . . ?
O11 S4 O10 Na2 180.001(0) 2 . . 2 ?
O4 S2 O4 Na3 -52.2(9) 3_675 . . 2_665 ?
O4 S2 O4 Na3 52.2(9) 2_765 . . . ?
O4 S2 O4 Na3 178.13(9) 3_675 . . . ?
O4 S2 O4 Na3 -178.13(9) 2_765 . . 2_665 ?
O4 S2 O4 Na4 63.0(4) 3_675 . . 2_665 ?
O4 S2 O4 Na4 -63.0(4) 2_765 . . 2_665 ?
O4 S2 O4 O3 63.0(4) 3_675 . . . ?
O4 S2 O4 O3 -63.0(4) 2_765 . . . ?
O4 S2 O3 Na4 119.999(1) 2_765 . . 2_665 ?
O4 S2 O3 Na4 0.001(0) 3_675 . . 1_665 ?
O4 S2 O3 Na4 -0.001(0) . . . 2_665 ?
O4 S2 O3 Na4 -120.001(0) 3_675 . . 2_665 ?
O4 S2 O3 Na4 -119.999(1) 2_765 . . 1_665 ?
O4 S2 O3 Na4 0.000(0) 2_765 . . 3_665 ?
O4 S2 O3 Na4 120.000(1) 3_675 . . 3_665 ?
O4 S2 O3 Na4 -120.000(1) . . . 3_665 ?
O4 S2 O3 Na4 120.000(0) . . . 1_665 ?
O4 S2 O3 O4 120.000(1) 3_675 . . 2_765 ?
O4 S2 O3 O4 120.000(1) 2_765 . . . ?
O4 S2 O3 O4 -120.000(1) . . . 2_765 ?
O4 S2 O3 O4 120.000(2) . . . 3_675 ?
O4 S2 O3 O4 -120.000(1) 2_765 . . 3_675 ?
O4 S2 O3 O4 -120.000(1) 3_675 . . . ?
O5 S2 O5 Na3 -172.88(7) 2_765 . . 2_665 ?
O5 S2 O5 Na3 172.88(7) 3_675 . . . ?
O5 S2 O5 Na3 46.1(13) 3_675 . . 2_665 ?
O5 S2 O5 Na3 -46.1(13) 2_765 . . . ?
O5 S2 O5 Na2 70.5(7) 2_765 . . 2_665 ?
O5 S2 O5 Na2 -70.5(7) 3_675 . . 2_665 ?
O5 S2 O6 Na2 120.000(1) 2_765 . . 1_665 ?
O5 S2 O6 Na2 -120.001(1) 2_765 . . 2_665 ?
O5 S2 O6 Na2 -0.001(0) . . . 2_665 ?
O5 S2 O6 Na2 119.998(0) 3_675 . . 2_665 ?
O5 S2 O6 Na2 -120.000(1) . . . 1_665 ?
O5 S2 O6 Na2 -0.001(0) 3_675 . . 1_665 ?
O5 S2 O6 Na2 -120.001(1) 3_675 . . 3_665 ?
O5 S2 O6 Na2 0.000(1) 2_765 . . 3_665 ?
O5 S2 O6 Na2 120.000(1) . . . 3_665 ?
O6 S2 O5 Na3 -116.6(7) . . . . ?
O6 S2 O5 Na3 116.6(7) . . . 2_665 ?
O6 S2 O5 Na2 0.001(0) . . . 2_665 ?
O3 S2 O4 Na3 115.2(5) . . . . ?
O3 S2 O4 Na3 -115.2(5) . . . 2_665 ?
O3 S2 O4 Na4 0.001(0) . . . 2_665 ?
O8 S3 O7 Na4 120.0 2_655 . . 8 ?
O8 S3 O7 Na4 0.000(1) 3_665 . . 7_665 ?
O8 S3 O7 Na4 120.000(1) . . . 7_665 ?
O8 S3 O7 Na4 -119.999(1) 3_665 . . 8 ?
O8 S3 O7 Na4 -120.000(0) 2_655 . . 7_665 ?
O8 S3 O7 Na4 0.001(1) . . . 8 ?
O8 S3 O7 Na4 120.000(1) 3_665 . . 9_655 ?
O8 S3 O7 Na4 -120.000(1) . . . 9_655 ?
O8 S3 O7 Na4 0.000(1) 2_655 . . 9_655 ?
O8 S3 O8 Na3 1(2) 3_665 . . . ?
O8 S3 O8 Na3 94.18(12) 2_655 . . . ?
O8 S3 O8 Na3 -94.18(12) 3_665 . . 2_655 ?
O8 S3 O8 Na3 -1(2) 2_655 . . 2_655 ?
O8 S3 O8 Na4 175.47(8) 2_655 . . . ?
O8 S3 O8 Na4 -82(2) 2_655 . . 3 ?
O8 S3 O8 Na4 82(2) 3_665 . . . ?
O8 S3 O8 Na4 -175.47(8) 3_665 . . 3 ?
O12 S4 O10 Na2 0.000(1) 8_556 . . 2 ?
O12 S4 O10 Na2 59.999(0) 3 . . . ?
O12 S4 O10 Na2 -0.001(1) 9_556 . . 3 ?
O12 S4 O10 Na2 -60.001(1) 2 . . . ?
O12 S4 O10 Na2 59.999(0) 2 . . 3 ?
O12 S4 O10 Na2 179.999(2) 3 . . 3 ?
O12 S4 O10 Na2 180.000(1) . . . . ?
O12 S4 O10 Na2 -0.001(1) 7_556 . . . ?
O12 S4 O10 Na2 180.000(1) 2 . . 2 ?
O12 S4 O10 Na2 119.999(1) 8_556 . . . ?
O12 S4 O10 Na2 -60.000(0) 3 . . 2 ?
O12 S4 O10 Na2 -120.001(0) 9_556 . . . ?
O12 S4 O10 Na2 -60.000(1) . . . 3 ?
O12 S4 O10 Na2 119.999(1) 7_556 . . 3 ?
O12 S4 O10 Na2 120.000(1) 9_556 . . 2 ?
O12 S4 O10 Na2 -120.000(1) 7_556 . . 2 ?
O12 S4 O10 Na2 60.001(1) . . . 2 ?
O12 S4 O10 Na2 -120.001(1) 8_556 . . 3 ?
O12 S4 O10 O12 -120.001(4) 3 . . . ?
O12 S4 O10 O12 179.999(3) 7_556 . . . ?
O12 S4 O10 O12 60.000(4) 7_556 . . 2 ?
O12 S4 O10 O12 60.000(5) 8_556 . . 3 ?
O12 S4 O10 O12 -119.999(3) . . . 2 ?
O12 S4 O10 O12 119.999(4) 2 . . . ?
O12 S4 O10 O12 59.999(3) 9_556 . . . ?
O12 S4 O10 O12 180.000(3) 8_556 . . 2 ?
O12 S4 O10 O12 -120.000(5) 2 . . 3 ?
O12 S4 O10 O12 -60.001(5) 8_556 . . . ?
O12 S4 O10 O12 180.000(6) 9_556 . . 3 ?
O12 S4 O10 O12 120.001(6) . . . 3 ?
O12 S4 O10 O12 -60.000(6) 7_556 . . 3 ?
O12 S4 O10 O12 120.000(3) 3 . . 2 ?
O12 S4 O10 O12 -60.000(3) 9_556 . . 2 ?
O12 S4 O12 Na1 179.999(3) 2 . . 1_445 ?
O12 S4 O12 Na1 180.000(5) 3 . . 3 ?
O12 S4 O12 Na1 73(3) 2 . . 3 ?
O12 S4 O12 Na1 -73(3) 3 . . 1_445 ?
O12 S4 O12 Na1 -107(3) 8_556 . . 3 ?
O12 S4 O12 Na1 -0.001(3) 8_556 . . 1_445 ?
O12 S4 O12 Na1 0.000(5) 9_556 . . 3 ?
O12 S4 O12 Na1 107(3) 9_556 . . 1_445 ?
O12 S4 O12 Na2 172(3) 8_556 . . 3 ?
O12 S4 O12 Na2 -98.5(7) 2 . . 2 ?
O12 S4 O12 Na2 98.5(7) 3 . . 3 ?
O12 S4 O12 Na2 8(3) 3 . . 2 ?
O12 S4 O12 Na2 -172(3) 9_556 . . 2 ?
O12 S4 O12 Na2 81.5(7) 8_556 . . 2 ?
O12 S4 O12 Na2 -81.5(7) 9_556 . . 3 ?
O12 S4 O12 Na2 -8(3) 2 . . 3 ?
O12 S4 O12 O10 126.5(16) 8_556 . . . ?
O12 S4 O12 O10 -53.5(16) 2 . . . ?
O12 S4 O12 O10 -126.5(16) 9_556 . . . ?
O12 S4 O12 O10 53.5(16) 3 . . . ?
O12 S4 O12 O12 107(3) 9_556 . . 8_556 ?
O12 S4 O12 O12 73(3) 2 . . 9_556 ?
O12 S4 O12 O12 -107(3) 8_556 . . 9_556 ?
O12 S4 O12 O12 180.000(2) 2 . . 8_556 ?
O12 S4 O12 O12 -73(3) 3 . . 8_556 ?
O12 S4 O12 O12 180.000(9) 3 . . 9_556 ?
O12 O10 O12 S4 -44.0(7) 3 . . . ?
O12 O10 O12 S4 44.0(7) 2 . . . ?
O12 O10 O12 Na1 64(2) 3 . . 1_445 ?
O12 O10 O12 Na1 -152.2(10) 3 . . 3 ?
O12 O10 O12 Na1 -64(2) 2 . . 3 ?
O12 O10 O12 Na1 152.2(10) 2 . . 1_445 ?
O12 O10 O12 Na2 84.6(7) 3 . . 2 ?
O12 O10 O12 Na2 -172.6(6) 3 . . 3 ?
O12 O10 O12 Na2 -84.6(7) 2 . . 3 ?
O12 O10 O12 Na2 172.6(6) 2 . . 2 ?
O12 O10 O12 O12 5(2) 2 . . 9_556 ?
O12 O10 O12 O12 -5(2) 3 . . 8_556 ?
O12 O10 O12 O12 -83.3(11) 3 . . 9_556 ?
O12 O10 O12 O12 83.3(11) 2 . . 8_556 ?
